# Tunable resonance transmission modes in hybrid heterostructures based on porous silicon

- Karina S Pérez
^{1}Email author, - J Octavio Estevez
^{1}, - Antonio Méndez-Blas
^{1}, - Jesús Arriaga
^{1}, - Gabriela Palestino
^{2}and - Miguel E Mora-Ramos
^{3}

**7**:392

https://doi.org/10.1186/1556-276X-7-392

© Pérez et al; licensee Springer. 2012

**Received: **30 April 2012

**Accepted: **13 July 2012

**Published: **13 July 2012

## Abstract

In this work, we report the experimental results and theoretical analysis of strong localization of resonance transmission modes generated by hybrid periodic/quasiperiodic heterostructures (HHs) based on porous silicon. The HHs are formed by stacking a quasiperiodic Fibonacci (FN) substructure between two distributed Bragg reflectors (DBRs). FN substructure defines the number of strong localized modes that can be tunable at any given wavelength and be unfolded when a partial periodicity condition is imposed. These structures show interesting properties for biomaterials research, biosensor applications and basic studies of adsorption of organic molecules. We also demonstrate the sensitivity of HHs to material infiltration.

## Keywords

## Background

Photonic crystals are attractive optical materials to control and manipulate the flow of light. A periodic dielectric system (multilayered), typically consisting of two alternated dielectric materials with periodic variation of refractive index (*n*), is the simplest photonic crystal (PC) [1]. The propagation of electromagnetic radiation in PCs is forbidden in specific wavelength ranges (photonic band gaps or PBGs) because the light wave is scattered at the layers’ interfaces, so the multiple-scattered waves interfere destructively into the material [2]. The behavior of light in a periodic scattering media can be described by Bloch states [3]. In addition, localized modes can appear into the PBGs by breaking the periodicity of the dielectric multilayer, i.e., by introducing a defect into a PC [4] that allows a narrow range of light wave frequencies to propagate through the whole structure. Physically, the defect is a single layer with different optical parameters (refractive index or thickness) or a completely different multilayer substructure [5]. Novel applications to optical devices, such as all-optical circuit, dielectric mirrors, Fabry-Perot filters, distributed feedback lasers, etc., have been proposed for the above-mentioned structures with localized modes. However, not only PCs based on periodic or periodical structures with defects are of interest but also deterministic aperiodic systems or quasicrystals because of their unexpected optical features [6–10]. The quasicrystals can be considered as a class of complex dielectric structures between ordered crystals and fully random structures. These structures show PBGs, but they are non-periodic multilayer structures. The quasicrystal structures are formed of layers with optical parameters that obey deterministic rules [11]. The Fibonacci and Thue-Morse mathematical sequences are two examples of numbers generated by deterministic rules. In order to associate these kinds of sequences to multilayer structures, it is necessary to define the so-called generators, i.e., initial layers with specific values of their optical properties.

Important applications for quasicrystal-type structures, such as band-edge lasing [12], optical frequency-selective filters [13], efficient nonlinear filters [14], bistability [15], and switching [16], have been suggested. In optical sensor applications based on PCs, the sensitivity is associated with the capacity for binding analyte molecules to the surface of the layers [17]. Porous silicon (PSi) has a great capacity of binding molecules at its surface due to its large specific superficial area (≥ 200 m^{2}/cm^{3}) [18]. The biocompatibility of the PSi [19] makes it a promising material to be used as a biosensor. PSi is a nanostructured material [20] considered as a mix of silicon and air with effective optical parameters, and its optical and structural features allow the fabrication of complex PCs [21–23]. Since PSi is obtained by electrochemical etching, and the porosity is directly related to the refractive index [24], it is possible to control its optical parameters by controlling the thickness and porosity by means of time and applied current during the process, respectively [25]. These features allow the fabrication of several types of one-dimensional (1D) PCs and the introduction of complex defect layers into a periodic multilayer structure. The strong confinement of electromagnetic fields within the engineered defect layers is an advantage offered by PCs because it is highly dependent on the refractive indices and thickness of each constituent layer; any change in these parameters is reflected as a change in the optical response. It is possible to achieve a spectral shift of the localized modes when a slight change of refractive index in some layers or on the whole structure is induced. Such displacements could be obtained by natural or thermal oxidation of the PSi structure or by introducing into the pores some specific substances. This advantage can be exploited particularly in biosensing applications due to its high sensitivity requirements compared to other sensors, which only use the weak evanescent field for sensing [26]. It is possible to obtain small spectral shifts in the reflectance or transmittance measures by introducing solutions or analytes into the pores of PSi, which can be monitored with exceptional precision. Numerous works have been published based on this idea, but only the simplest PSi structures (i. e. monolayers, distributed Bragg reflectors (DBRs), and several types of filters) have been used to study different molecular species as proteins [27, 28], DNA [29], solvents [30], neurons [31], etc. However, the optical features of PSi complex multilayer structures have not been explored widely for their application in the biosensing area. From this perspective, our interest lies on the fabrication of a highly efficient photonic structure for biosensing purposes. To achieve this goal, in this work, the fabrication of hybrid heterostructures (HHs) based on PSi is proposed. The HHs are a complex combination of the features of periodic and quasiperiodic photonic structures. The study of hybrid heterostructures has been approached in previous works by other authors but only in the theoretical aspect, and they not consider PSi nanostructures [32, 33]. It is the first experimental study of HHs based on Fibonacci (FN) sequences.

## Methods

^{ N }−(FN)

^{ M }−(DBR)

^{ N }[34]. The DBRs are formed by a periodic arrangement of two alternated layers,

*A*and

*B*

*N*times. The FN sequences are generated by the recursion relation

*F*

_{ M }=

*F*

_{M−1}+

*F*

_{M−2}where

*M*represents the order of the sequence (

*M*=2,3,4,…). It is possible to generate dielectric multilayered structures that follow the FN mathematical sequence of any order by choosing

*F*

_{0}=

*C*and

*F*

_{1}=

*CD*where

*C*and

*D*are two different layers. For example,

*F*

_{2}=

*CDC*

*F*

_{3}=

*CDCCD*

*F*

_{4}=

*CDCCDCDC*, and so on. The HHs present strongly localized transmission modes as a function of the design parameters and can be localized over a wide range of frequencies. The HHs based on PSi studied in this work were obtained by electrochemical etching from boron-doped silicon wafers (100)-oriented and 0.007 to 0.013

*Ω*cm resistivity. A small piece of silicon wafer was used as substrate for etching in an HF (40%) and ethanol (99.98%) solution in a volumetric ratio of 1:1. More details about the process can be found in reference [5]. In order to calculate the refractive index of each layer for a given current density, we use the effective medium approximation of the Bruggeman’s model [35]:

*ε*

_{PSi}) as a function of the dielectric constants of silicon (

*ε*

_{Si}) and air (

*ε*

_{air}), as well as porosity

*f*

_{p}. The values of

*f*

_{p}were calculated by the gravimetrical method. As the PSi layers consist of only two optical media, the

*ε*

_{PSi}value is intermediate between the

*ε*

_{Si}and

*ε*

_{air}values, weighed by the volume fraction 1−

*f*

_{p}and

*f*

_{p}, respectively, (in Equation 1 we take

*ε*

_{air}=1). Solving for

*ε*

_{PSi}in Equation 1, we obtain

*n*) and the extinction coefficient (

*k*) for dielectric materials (with exponential absorption), far from the absorption bands [36], by the equations

*a*

*b*

*c*

*d*, and

*e*. These parameters are adjusted to experimental values of

*n*and

*k*for crystalline silicon from reference [37]. For example, in Figure 1

*n*and

*k*are plotted for two different values of porosity (low and high) which correspond to the design parameters for the

*A*and

*B*layers (40% and 77% of porosity, respectively) of the DBRs mentioned above. In all the simulations, we consider Equations 3 and 4.

*λ*value around 1.0

*μ*m, the refractive index and thickness for layer

*A*is 1.4 and 178.5 nm, and for layer

*B*, 2.5 and 100 nm, respectively. The refractive indices for

*C*and

*D*layers are 1.6 and 2.2, and their thicknesses are 156.25 and 113.64 nm, respectively. In all these layers, the optical thickness

*nd*, where

*n*is the refractive index and

*d*is the physical thickness, has the constant value

*λ*/4 = 250 nm. A schematic of the structure with the sequence (DBR)

^{4}−(FN)

^{4}−(DBR)

^{4}is shown in Figure 2, in which it is possible to observe the formation of two optical modes corresponding to

*λ*/2 defects.

*M*= 3, 4, 5…), it presents one, two, or three resonance transmission modes, respectively. The number of resonances is in direct analogy with the FN sequence (see Table 1).

*N*= 4 in DBRs substructures was kept constant for all the structures.

**Fibonacci order, substructure, and sequence**

FN substructure | FN sequence and number | |
---|---|---|

Generators: | of defects Generators: | |

Order | F | F |

2 |
| 1 |

3 |
| 1 |

4 |
| 2 |

5 |
| 3 |

6 |
| 5 |

7 |
| 8 |

The reflectivity measurements of 1D photonic crystals based on PSi structures were carried out in an Agilent spectrophotometer (Cary 5000 UV-VIS-NIR, Agilent Technologies, Santa Clara, CA, USA), with the specular reflectance accessory (VASRA). All the spectra were measured at an angle of incidence of 20°. Reflectivity measurements were carried out with a p-polarized beam. The experimental results were compared with those given by the theory.

### Theoretical model

**k**=

**k**

_{∥}+

**k**

_{ z }, there are two independent EM modes: transverse-magnetic (TM) modes and transverse electric (TE) modes. The electric (magnetic) field for the TE (TM) mode is perpendicular to the plane defined by the wave vector and the direction of periodicity. Using the transfer matrix formalism, we can relate the amplitudes of the fields ${E}_{\mathrm{j\mu}}^{+}$ and $\left({E}_{\mathrm{j\mu}}^{-}\right)$ in the

*j*−

*th*layer of the system to the amplitudes of the field in the (

*j*+ 1)−

*th*layer according to

*j*, with polarization

*μ*(

*μ*=

*s*

*p*) traveling to the right (left). For the case considered in this work, the total transfer matrix of the system can be written as a product of matrices of the type [39]

where ${q}_{\mathrm{j\mu}}={k}_{j}^{2}/{k}_{\mathrm{jz}}$ for *p*-polarization and *q*_{
jμ
}=(*k*_{
jz
}) for *s*-polarization; *ϕ*_{
j
} = *k*_{
jz
}*d*_{
j
}*k*_{
j
} = (*ω*/ *c*) *n*_{
j
}*k*_{
jz
}is the component of the wave vector along the growth direction of the system in the *j*− *th* layer given by ${k}_{\mathrm{jz}}\phantom{\rule{1em}{0ex}}=\phantom{\rule{1em}{0ex}}\sqrt{{k}_{j}^{2}-{k}_{\parallel}^{2}}$; and ${n}_{j}\phantom{\rule{1em}{0ex}}=\phantom{\rule{1em}{0ex}}\sqrt{{\epsilon}_{j}}$ is the complex refractive index. The reflectivity of the system is given in terms of the matrix elements of the total transfer matrix according to $R={\left|{M}_{21}/{M}_{11}\right|}^{2}$. We have implemented a realistic transfer matrix approach by considering the wavelength dependence of the refractive index as well as the optical absorption. Absorption is a very important parameter, especially when considering the visible region of the electromagnetic spectrum.

## Results and discussion

^{4}−(FN)

^{3}−(DBR)

^{4}presents one localized transmission mode at 988 nm with 19.7 nm of full width at half-maximum (FWHM). The localized mode is produced by the two adjacent

*λ*/4 layers, in this case, two

*C*layers in the FN substructure. The HH based on the fourth-order FN substructure (Figure 3b) presents two localized modes at 977 and 1,112.4 nm with a FWHM of 15.7 and 22.7 nm, respectively. The first localized transmission mode is produced again by two

*C*layers in the FN substructure. However, the second defect is produced by a

*C*layer from an FN substructure adjacent to an

*A*layer from the DBR substructure. Even though the refractive index and the thickness for both layers are different, their optical thickness is the same (

*nd*=

*λ*/4), so the

*λ*/2 condition is kept. Furthermore, in this case, the condition of periodicity is met before and after the defect. In Figure 3c, the fifth order of the FN substructure between the DBRs produces three resonant modes at 934.5, 1,036.3, and 1,160.8 nm with FWHMs of 13.2, 14.8, and 23.6, respectively. In this case, all the localized modes are due to three pairs of

*C*layers in the FN substructure. For HHs corresponding to the upper order of FN substructures, similar defects are found, and the number of defects follows the numerical Fibonacci’s sequence (see Table 1). The optical modes can be designed to appear at almost any wavelength because they depend on the optical thickness, i.e., we can design specific PSi structures with the correct refractive indices and thicknesses to match any electromagnetic region. Theoretical simulations of the same HHs are also plotted in Figure 3 (dotted line). In these simulations, we took the values of refractive index and thickness mentioned in the ‘Methods’ section but considering ±0.05 deviation in the refractive index values. From this figure, the excellent agreement with the experimental results can be seen, which gives us certainty on the theoretical modeling. This model takes into account the

*n*(

*λ*) and

*k*(

*λ*) dependence for each layer.

^{4}−(FN)

^{4}−(DBR)

^{4}shown in Figure 3b. The first modification consists of adding or removing layers from the FN substructure; in any case, the Fibonacci sequence is lost. However, the spectral positions where the resonances appear can be changed by this modification. In Figure 5, the effect of removing some layers from the FN substructure can be observed. The original structure from Figure 3b is shown again in Figure 5a for reference. From the (DBR)

^{4}−(FN)

^{4}−(DBR)

^{4}structure, the two last layers from the FN substructure were removed, and the resulting structure is now (DBR)

^{4}−(CDCCDC)−(DBR)

^{4}. In Figure 5b, it can be seen that the two resonances are localized at 960.7 and 1,143.6 nm with FWHMs of 17.4 and 28.6, respectively, so the range between the resonances has increased to 182.9 nm, the range being 135.4 nm before modifying the FN sequence (Figure 5a). Moreover, the addition of a pair of DC layers to the end of the FN substructure results in the structure (DBR)

^{4}−(FN)

^{4}DC−(DBR)

^{4}. Figure 5c shows the resulting reflectance spectra after the last modification. Now, the optical resonances appear at 1,013.9 and 1,118.4 nm, so the new range between the two resonances is 101.5 nm, i.e., the difference of the two resonances’ spectral position has decreased, compared to original HHs. This result can be explained taking into account the interaction between the defect modes. The larger the physical distance between the defect layers, the weaker is the interaction of the eigenmodes so that they can appear at the nearest frequencies when there is a very long distance between defects layers. On the other hand, when the distance between defects is short, the interaction of the eigenmodes increases, but they cannot appear at the same energy or frequency in the optical spectra. Consequently, the localized modes in the reflectance spectra appear more separated [40]. These important features prove the flexibility of the structures and their capacity to localize the resonant modes at almost any wavelength as a function of the design parameters. This tunability can be exploited in optical devices, particularly in the biosensing area.

^{4}−(FN)

^{4}−(DBR)

^{4}, we obtain (DBR)

^{4}−(FN)

^{4}−(DBR)

^{4}−(FN)

^{4}−(DBR)

^{4}, and the resulting reflectance spectra of the new structure (see Figure 6) show twofold of each resonance mode that appears in the original structure in Figure 3b. A threefold splitting can be obtained by repeating three times the unit cell; fourfold splitting would correspond to four times, and so on.

The effective refractive index in PSi is the result of a homogeneous mixture of air and silicon, so any material infiltration into the pores displaces off part of the air. Consequently, a red- or blueshift could be expected in the optical reflectance spectra due to a partial change of the optical parameters. The same effect is expected in monolayers and multilayers or even in more complex PSi structures. So, red- or blueshift can be monitored in order to estimate the sensitivity of the structures. To achieve this in multilayered structures, it is preferable to have strong localized modes in order to follow more easily the spectral displacements. The HHs developed in this work have the strong localized modes needed, but they are observed in very complex structures. However, we want to demonstrate that these complex structures make them more sensitive to material infiltration, in particular, when biological molecules are placed into the pores of HHs based on PSi. In order to know the feasibility of the HHs to be used as biosensors, 3-aminopropyltriethoxysilane (APTES) molecule was attached to the internal surface of the structure [41]. To do this, it is necessary to follow a specific process described here: (1) HHs based on PSi were thermally stabilized at 900°C under oxygen flow; (2) APTES silanization was done in a 5% solution with toluene during 1.5 h; (3) the samples were rinsed with toluene and dried under nitrogen flow, and finally, (4) samples were baked in an oven at 110°C for 15 min. The procedure to silane’s modification is well described elsewhere [42].

^{4}−(FN)

^{4}−(DBR)

^{4}HHs in the three stages of the procedure can be seen clearly. Figure 7a shows the reflectance spectra of the sample as prepared. The thermal stabilization of the samples in oxygen atmosphere produces a partial transformation of the silicon filaments to silicon dioxide. The refractive index of silicon dioxide is lower with respect to silicon; therefore, a decrease in the effective refractive index of the layers [43] in the HHs can be detected by a large displacement of the resonant modes to short wavelengths. This blueshift is observed in Figure 7b and compared with a sample as prepared in Figure 7a. Moreover, the infiltration of biological molecules into the pores produces a redshift because the APTES molecules displace the air from the pores. The redshift of resonances can be easily detected by optical reflectance. As can be seen in Figure 7c, a redshift of 44.3 nm was obtained with respect to the oxidized sample (Figure 7b). Even by using low concentration of APTES (approximately 5%), the spectral displacements are larger than the previously reported ones in PSi structures that were infiltrated with several molecular species [44, 45]. This effect can be attributed to the large specific surface area of the PSi that allows us to have a large quantity of available sites for chemical binding. This idea is based on the saturation curves obtained for APTES in micro- and mesoporous structures reported in reference [46] and confirmed in our samples (not shown for brevity). In order to compare the sensitivity of the APTES infiltration in HHs and the structure given in reference [45], we have calculated the

*ΔE*(in electron volt) from the spectral position of the resonance modes before and after the APTES infiltration. In that reference,

*ΔE*∼ 0.27 eV for structures designed at 830 nm. In our case,

*ΔE*=0.053 eV for

*λ*=1.0

*μ*m, according to the pore size criteria given above. An important characteristic that the HHs offer is the possibility to generate strong localized transmission modes that allow us to better monitor their spectral displacements even at a low concentration of analyte.

Theoretical simulation is also presented in Figure 7 (dashed line). In this case, unlike the first simulations and as a result of changes in the effective refractive index produced by thermal oxidation and APTES infiltration, we introduced a constant *Δ* *n*_{
i
} in order to reproduce the best possible experimental reflectance, where *i* corresponds to layers *A*, *B*, *C* and *D*. The values of *Δ* *n*_{
i
} were adjusted, taking into account that the silicon dioxide grows at the expense of silicon (reducing the effective refractive index) and APTES displaces the air from the pores (increasing the effective refractive index). We found that the values of *Δ* *n*_{
i
} induced by the APTES attachment on the oxidized layers is ≤0.09 for each layer. Figure 7 shows a good agreement between the experimental and calculated spectra. The simulation of the optical spectra, based on experimental data of the HHs structures with the molecule infiltration, could give us a quantitative analysis method for material infiltration even at a very low concentration.

## Conclusions

In conclusion, we have been able to demonstrate the fabrication of hybrid heterostructures consisting of dielectric multilayers of distributed Bragg reflectors and Fibonacci type. Even considering the complexity of the HHs and the multiple factors involved in PSi formation, we obtain a very high quality and reproducibility in PSi multilayers in our experimental setup. The possibility to localize resonant modes and tuning them has been proven. Unfolding of resonant modes can be generated by repeating periodically the hybrid structure. The theoretical model is in good agreement with the experimental data, so it could be used to estimate changes in optical responses of chemically modified structures. Such hybrid heterostructures can be very promising in the field of optoelectronics, optical communications [47], and biosensors [48].

## Declarations

### Acknowledgements

This work has been partially supported by CONACyT under project No. 101486 and by PROMEP “Red Temática”. SEM images: Instituto Potosino de Investigación Científica y Tecnológica A. C. (IPICYT).

## Authors’ Affiliations

## References

- Joannopoulos JD, Meade RD, Winn JN:
*Phothonic Crystals: Molding the Flow of Light*. New Jersey: Princeton University Press; 1995.Google Scholar - Prather DW, Shi S, Sharkawi S, Murakowski J, Schneider GJ:
*Photonic Crystals: Theory, Applications, and Fabrication*. New Jersey: Wiley; 2009.Google Scholar - Kittel C:
*Introduction to Solid State Physics*. New York: Wiley; 1996.Google Scholar - Ghulinyan M, Oton CJ, Gaburro Z, Bettotti P, Pavesi L: Porous silicon free-standing coupled microcavities.
*Appl Phys Lett*2003, 82: 1550–1552. 10.1063/1.1559949View ArticleGoogle Scholar - Pérez K, Estevez JO, Méndez-Blas A, Arriaga J: Localized defect modes in dual-periodical multilayer structures based on porous silicon.
*J Opt Soc Am: B*2012, 29: 538–542. 10.1364/JOSAB.29.000538View ArticleGoogle Scholar - Rammal R, Tolouse G: Random walks on fractal structures and percolation clusters.
*J Phys Lett*1983, 44: L13—L22.Google Scholar - Kohmoto M, Shuterland B: Critical wave functions and a Cantor-set spectrum of a one-dimensional quasicrystal model.
*Phys Rev B*1987, 35: 1020–1033. 10.1103/PhysRevB.35.1020View ArticleGoogle Scholar - Gellerman W, Kohmoto M, Shuterland B, Taylor PC: Localization of light waves in Fibonacci dielectric multilayers.
*Phys Rev Lett*1994, 72: 633–636. 10.1103/PhysRevLett.72.633View ArticleGoogle Scholar - Fujita N, Niizeki K: Electronic properties of ternary quasicrystals in one dimension.
*Phys Rev B*2001, 64: 144207.View ArticleGoogle Scholar - Iglói F, Turban L, Rieger H: Anomalous diffusion in aperiodic environments.
*Phys Rev E*1999, 59: 1465–1474. 10.1103/PhysRevE.59.1465View ArticleGoogle Scholar - Fujiwara T, Owaga T:
*Quasicrystals*. Berlin: Springer-Verlag; 1990.View ArticleGoogle Scholar - Sibilia C, Nefedov I, Scalora M, Bertolitti M: Electromagnetic mode density for finite quasi-periodic structures.
*JOSA B*1998, 15: 1947–1952. 10.1364/JOSAB.15.001947View ArticleGoogle Scholar - Ali NB, Trabelsi Y, Kanzari M: Stop band filter by using hybrid quasi-periodic one dimensional photonic crystal in microwave domain.
*IJMOT*2009, 4: 195–204.Google Scholar - Sibilia C: Optical properties of quasiperiodic (fractals) one-dimensional structures. In
*Nanoscale linear and nonlinear optics: July 2–14, 2000; Sicily*. Edited by: Bertolotti M. College Park: AIP Conf Proc; 2001:220–220.Google Scholar - Bertolotti M, Masciulli P, Ranieri P, Sibilia C: Optical bistability in a nonlinear Cantor corrugated waveguide.
*JOSA B*1996, 13: 1517–1525. 10.1364/JOSAB.13.001517View ArticleGoogle Scholar - Scalora M, Dowling JP, Bowden CM, Bloemer M: Optical limiting and switching of ultrashort pulses in nonlinear photonic band gap materials.
*Phys Rev Lett*1994, 73: 1368–1371. 10.1103/PhysRevLett.73.1368View ArticleGoogle Scholar - Ouyang H, Fauchet PM: Biosensing using porous silicon photonic bandgap structures. In
*Photonic Crystals and Photonic Crystal Fibers for Sensing Applications*. Edited by: Du HH. Bellingham: SPIE Optics East; 2005:08–08.Google Scholar - DeLouise LA, Miller BL: Quantitative assessment of enzyme immobilization capacity in porous silicon.
*Anal Chem*2004, 76: 6915–6920. 10.1021/ac0488208View ArticleGoogle Scholar - Ghoshal S, Mitra D, Roy S: Dutta Majumder D:Biosensors and biochips for nanomedical applications: a review.
*Sens Transducers*2010, 113: 1–17.Google Scholar - Chan S, Fauchet PM: Tunable, narrow, and directional luminescence from porous silicon light emitting devices.
*Appl Phys Lett*1999, 75: 274–276. 10.1063/1.124346View ArticleGoogle Scholar - Estevez JO, Arriaga J, Méndez Blas A, Agarwal V: Omnidirectional photonic bandgaps in porous silicon based mirrors with a Gaussian profile refractive index.
*Appl Phys Lett*2008, 93: 191915. 10.1063/1.3028073View ArticleGoogle Scholar - Lin VS-Y, Motesharei K, Dancil K-PS, Sailor MJ, Ghadiri MR: A porous silicon-based optical interferometric biosensor.
*Science*1997, 278: 840–843. 10.1126/science.278.5339.840View ArticleGoogle Scholar - Escorcia-Garcia J, Agarwal V, Parmananda P: Noise mediated regularity of porous silicon nanostructures.
*Appl Phys Lett*2009, 94: 133103. 10.1063/1.3104854View ArticleGoogle Scholar - Canham LT: Silicon quantum wire array fabrication by electrochemical and chemical dissolution of wafers.
*Appl Phys Lett*1990, 57: 1046–1048. 10.1063/1.103561View ArticleGoogle Scholar - Agarwal V, del Río JA: Tailoring the photonic band gap of a porous silicon dielectric mirror.
*Appl Phys Lett*2003, 82: 1512–1514. 10.1063/1.1559420View ArticleGoogle Scholar - Nightingale JR: Optical biosensors: SPARROW biosensor and biophotonic crystal-based fluorecence enhancement.
*PhD thesis*. West Vinginia University, College of Engineering and Mineral Resources; 2008.Google Scholar - Dancil K-PS, Greiner DP, Sailor MJ: A porous silicon optical biosensor: detection of reversible binding of IgG to a protein A-modified surface.
*J Am Chem Soc*1999, 121: 7925–7930. 10.1021/ja991421nView ArticleGoogle Scholar - Zangooie S, Bjorklund R, Arwin H: Protein adsorption in thermally oxidized porous silicon layers.
*Thin Solid Films*1998, 313: 825–830.View ArticleGoogle Scholar - Rong G, Weiss SM: Biomolecule size-dependent sensitivity of porous silicon sensors.
*Phys Status Solidi A*2009, 206: 1365–1368. 10.1002/pssa.200881097View ArticleGoogle Scholar - Chapron J, Alekseev SA, Lysenko V, Zaitsev VN, Barbier D: Analysis of interaction between chemical agents and porous Si nanostructures using optical sensing properties of infra-red Rugate filters.
*Sensors and Actuators B*2007, 120: 706–711. 10.1016/j.snb.2006.03.038View ArticleGoogle Scholar - Moxon KA, Hallman S, Aslani A, Kalkhoran NM, Lelkes PI: Bioactive properties of nanostructured porous silicon for enhancing electrode to neuron interfaces.
*J Biomater Sci Polymer Edn*2007, 18: 1263–1281. 10.1163/156856207782177882View ArticleGoogle Scholar - Dong J-W, Hang P: Wang H-Z: Broad omnidirectional reflection band forming using the combination of Fibonacci quasi-Periodic and periodic one-dimensional photonic crystals.
*Chin Phys Lett*2003, 20: 1963–1965. 10.1088/0256-307X/20/11/017View ArticleGoogle Scholar - Ali N, Kanzari M: Designing of stop band filters using hybrid periodic/quasi-periodic one-dimensional photonic crystals in microwave domain.
*Phys Stat Solidi A*2011, 208: 161–171. 10.1002/pssa.200925531View ArticleGoogle Scholar - Escorcia-Garcia J, Duque CA, Mora-Ramos ME: Optical properties of hybrid periodic/quasiregular dielectric multilayers.
*Superlattices and Microstructures*2011, 49: 203–208. 10.1016/j.spmi.2010.08.006View ArticleGoogle Scholar - Pap AE, Kordás K, Vähäkangas J, Uusimäki A, Leppävuori S, Pilon L, Szatmári S: Optical properties of porous silicon. Part III: comparison of experimental and theoretical results.
*Opt Mater*2006, 28: 506–513. 10.1016/j.optmat.2005.02.006View ArticleGoogle Scholar - Bosch S, Ferré-Borrull J, Sancho-Parramon J: A general-purpose software for optical characterization of thin films: specific features for microelectonic applications.
*Solid-State Electronics*2001, 45: 703–709. 10.1016/S0038-1101(01)00092-2View ArticleGoogle Scholar - Palik ED:
*Handbook of Optical Constants of Solids*. San Diego: Academic Press; 1998.Google Scholar - Yeh P:
*Optical Waves in Layered Media*. New Jersey: Wiley VCH; 1998.Google Scholar - Arriaga J, Saldan̄a XI: Band structure and reflectivity of omnidirectional Si-based mirrors with a Gaussian profile refractive index.
*J Appl Phys*2006, 100: 044911. 10.1063/1.2336078View ArticleGoogle Scholar - Qin Q, Lu H, Zhu SN, Yuan CS, Zhu YY, Ming NB: Resonance transmission modes in dual-periodical dielectric multilayer films.
*Appl Phys Lett*2003, 82: 4654–4656. 10.1063/1.1587880View ArticleGoogle Scholar - Palestino G, Martin M, Agarwal V, Legros R, Cloitre T, Zimányi L, Gergelly C: Detection and light enhancement of glucose oxidase adsorbed on porous silicon microcavities.
*Phys Status Solidi C*2009, 6: 1624–1628. 10.1002/pssc.200881006View ArticleGoogle Scholar - Palestino G, Agarwal V, Aulombard R, Pérez E, Gergely C: Biosensing and protein fluorescence enhancement by functionalized porous silicon devices.
*Langmuir*2008, 24: 13765–13771. 10.1021/la8015707View ArticleGoogle Scholar - Steinem C, Janshoff A, Lin VS-Y, Völker NH, Reza Ghadiri: DNA hybridization-enhanced porous silicon corrosion: mechanistic investigations and prospect for optical interferometric biosensing.
*Tetrahedron*2004, 60: 11259–11267. 10.1016/j.tet.2004.06.130View ArticleGoogle Scholar - Palestino G, Agarwal V, Garcá DB, Legros R, Pérez E, Gergelly C: Optical characterization of porous silicon microcavities for glucose oxidase biosensing. In
*Biophotonics: Photonic Solutions for Better Health Care. Strasbourg.*. Edited by: Popp J, Drexler W, Tuchin VV, Matthews DL. Proc SPIE; 2008:69911Y-1.View ArticleGoogle Scholar - Ouyang H, DeLouise LA, Miller BL, Fauchet PM: Label-free quantitative detection of protein using macroporous silicon photonic bandgap biosensors.
*Anal Chem*2007, 79: 1502–1506. 10.1021/ac0608366View ArticleGoogle Scholar - Ouyang H, Striemer CC, Fauchet PM: Quantitative analysis of the sensitivity of porous silicon optical biosensors.
*Appl Phys Lett*2006, 88: 163108. 10.1063/1.2196069View ArticleGoogle Scholar - Lee H-Y, Yao T: Design and evaluation of omnidirectional one-dimensional photonic crystals.
*J Appl Phys*2003, 93: 819–830. 10.1063/1.1530726View ArticleGoogle Scholar - Lin VS-Y, Motesharei K, Dancil K-PS, Sailor MJ, Ghadiri MR: A porous silicon-based optical interferometric biosensor.
*Science*1997, 278: 840–843. 10.1126/science.278.5339.840View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.